General

Property | Temperature | Value |
---|---|---|

Density | 20.0 °C | 7.94 g/cm³ Show Material materials with Density of 7.94 g/cm³ |

Mechanical

Property | Temperature | Value | Comment |
---|---|---|---|

Elastic modulus | -100.0 °C | 201 GPa Show Material materials with Elastic modulus of 201 GPa | |

20.0 °C | 194 - 197 GPa Show Material materials with Elastic modulus of 194 - 197 GPa | ||

100.0 °C | 189 - 191 GPa Show Material materials with Elastic modulus of 189 - 191 GPa | ||

200.0 °C | 183 - 184 GPa Show Material materials with Elastic modulus of 183 - 184 GPa | ||

300.0 °C | 177 GPa Show Material materials with Elastic modulus of 177 GPa | ||

400.0 °C | 170 GPa Show Material materials with Elastic modulus of 170 GPa | ||

500.0 °C | 162 - 163 GPa Show Material materials with Elastic modulus of 162 - 163 GPa | ||

600.0 °C | 155 - 156 GPa Show Material materials with Elastic modulus of 155 - 156 GPa | ||

700.0 °C | 148 - 149 GPa Show Material materials with Elastic modulus of 148 - 149 GPa | ||

800.0 °C | 141 GPa Show Material materials with Elastic modulus of 141 GPa | ||

900.0 °C | 134 GPa Show Material materials with Elastic modulus of 134 GPa | ||

1000.0 °C | 127 GPa Show Material materials with Elastic modulus of 127 GPa | ||

Elongation | 20.0 °C | 30 - 35 % Show Material materials with Elongation of 30 - 35 % | |

Poisson's ratio | 23.0 °C | 0.3 [-] Show Material materials with Poisson's ratio of 0.3 [-] | Typical for Austenitic Stainless Steel |

Shear modulus | 23.0 °C | 77 GPa Show Material materials with Shear modulus of 77 GPa | Typical for Austenitic Stainless Steel |

Tensile strength | 20.0 °C | 500 - 750 MPa Show Material materials with Tensile strength of 500 - 750 MPa | |

Yield strength Rp0.2 | 20.0 °C | 170 MPa Show Material materials with Yield strength Rp0.2 of 170 MPa | |

100.0 °C | 140 MPa Show Material materials with Yield strength Rp0.2 of 140 MPa | ||

200.0 °C | 115 MPa Show Material materials with Yield strength Rp0.2 of 115 MPa | ||

300.0 °C | 95 MPa Show Material materials with Yield strength Rp0.2 of 95 MPa | ||

400.0 °C | 85 MPa Show Material materials with Yield strength Rp0.2 of 85 MPa | ||

500.0 °C | 80 MPa Show Material materials with Yield strength Rp0.2 of 80 MPa | ||

550.0 °C | 75 MPa Show Material materials with Yield strength Rp0.2 of 75 MPa | ||

600.0 °C | 75 MPa Show Material materials with Yield strength Rp0.2 of 75 MPa | ||

700.0 °C | 75 MPa Show Material materials with Yield strength Rp0.2 of 75 MPa | ||

800.0 °C | 70 MPa Show Material materials with Yield strength Rp0.2 of 70 MPa | ||

900.0 °C | 50 MPa Show Material materials with Yield strength Rp0.2 of 50 MPa | ||

1000.0 °C | 20 MPa Show Material materials with Yield strength Rp0.2 of 20 MPa | ||

Unlock all property charts | |||

Yield strength Rp1.0 | 20.0 °C | 200 MPa Show Material materials with Yield strength Rp1.0 of 200 MPa | |

100.0 °C | 160 MPa Show Material materials with Yield strength Rp1.0 of 160 MPa | ||

200.0 °C | 135 MPa Show Material materials with Yield strength Rp1.0 of 135 MPa | ||

300.0 °C | 115 MPa Show Material materials with Yield strength Rp1.0 of 115 MPa | ||

400.0 °C | 105 MPa Show Material materials with Yield strength Rp1.0 of 105 MPa | ||

500.0 °C | 100 MPa Show Material materials with Yield strength Rp1.0 of 100 MPa | ||

550.0 °C | 95 MPa Show Material materials with Yield strength Rp1.0 of 95 MPa | ||

600.0 °C | 95 MPa Show Material materials with Yield strength Rp1.0 of 95 MPa | ||

Unlock all property charts |

Thermal

Property | Temperature | Value | Comment |
---|---|---|---|

Coefficient of thermal expansion | -100.0 °C | 1.36E-5 1/K Show Material materials with Coefficient of thermal expansion of 1.36E-5 1/K | |

20.0 °C | 1.46E-5 1/K Show Material materials with Coefficient of thermal expansion of 1.46E-5 1/K | ||

100.0 °C | 1.51E-5 - 1.54E-5 1/K Show Material materials with Coefficient of thermal expansion of 1.51E-5 - 1.54E-5 1/K | ||

200.0 °C | 1.57E-5 - 1.6E-5 1/K Show Material materials with Coefficient of thermal expansion of 1.57E-5 - 1.6E-5 1/K | ||

300.0 °C | 1.62E-5 - 1.65E-5 1/K Show Material materials with Coefficient of thermal expansion of 1.62E-5 - 1.65E-5 1/K | ||

400.0 °C | 1.66E-5 - 1.68E-5 1/K Show Material materials with Coefficient of thermal expansion of 1.66E-5 - 1.68E-5 1/K | ||

500.0 °C | 1.7E-5 - 1.72E-5 1/K Show Material materials with Coefficient of thermal expansion of 1.7E-5 - 1.72E-5 1/K | ||

600.0 °C | 1.74E-5 - 1.75E-5 1/K Show Material materials with Coefficient of thermal expansion of 1.74E-5 - 1.75E-5 1/K | ||

700.0 °C | 1.77E-5 - 1.79E-5 1/K Show Material materials with Coefficient of thermal expansion of 1.77E-5 - 1.79E-5 1/K | ||

800.0 °C | 1.8E-5 - 1.83E-5 1/K Show Material materials with Coefficient of thermal expansion of 1.8E-5 - 1.83E-5 1/K | ||

900.0 °C | 1.83E-5 - 1.86E-5 1/K Show Material materials with Coefficient of thermal expansion of 1.83E-5 - 1.86E-5 1/K | ||

1000.0 °C | 1.86E-5 - 1.9E-5 1/K Show Material materials with Coefficient of thermal expansion of 1.86E-5 - 1.9E-5 1/K | ||

Unlock all property charts | |||

Max service temperature, long | 500 - 700 °C Show Material materials with Max service temperature, long of 500 - 700 °C | ||

Melting point | 1230 - 1480 °C Show Material materials with Melting point of 1230 - 1480 °C | Typical for Austenitic Stainless Steel | |

Specific heat capacity | -100.0 °C | 440 J/(kg·K) Show Material materials with Specific heat capacity of 440 J/(kg·K) | |

20.0 °C | 460 - 472 J/(kg·K) Show Material materials with Specific heat capacity of 460 - 472 J/(kg·K) | ||

100.0 °C | 487 J/(kg·K) Show Material materials with Specific heat capacity of 487 J/(kg·K) | ||

200.0 °C | 503 J/(kg·K) Show Material materials with Specific heat capacity of 503 J/(kg·K) | ||

300.0 °C | 512 J/(kg·K) Show Material materials with Specific heat capacity of 512 J/(kg·K) | ||

400.0 °C | 520 J/(kg·K) Show Material materials with Specific heat capacity of 520 J/(kg·K) | ||

500.0 °C | 530 J/(kg·K) Show Material materials with Specific heat capacity of 530 J/(kg·K) | ||

600.0 °C | 541 J/(kg·K) Show Material materials with Specific heat capacity of 541 J/(kg·K) | ||

700.0 °C | 551 J/(kg·K) Show Material materials with Specific heat capacity of 551 J/(kg·K) | ||

800.0 °C | 559 J/(kg·K) Show Material materials with Specific heat capacity of 559 J/(kg·K) | ||

900.0 °C | 565 J/(kg·K) Show Material materials with Specific heat capacity of 565 J/(kg·K) | ||

1000.0 °C | 571 J/(kg·K) Show Material materials with Specific heat capacity of 571 J/(kg·K) | ||

Unlock all property charts | |||

Thermal conductivity | 20.0 °C | 11.5 - 12 W/(m·K) Show Material materials with Thermal conductivity of 11.5 - 12 W/(m·K) | |

100.0 °C | 13.1 W/(m·K) Show Material materials with Thermal conductivity of 13.1 W/(m·K) | ||

200.0 °C | 14.8 W/(m·K) Show Material materials with Thermal conductivity of 14.8 W/(m·K) | ||

300.0 °C | 16.4 W/(m·K) Show Material materials with Thermal conductivity of 16.4 W/(m·K) | ||

400.0 °C | 18.1 W/(m·K) Show Material materials with Thermal conductivity of 18.1 W/(m·K) | ||

500.0 °C | 19.6 W/(m·K) Show Material materials with Thermal conductivity of 19.6 W/(m·K) | ||

600.0 °C | 21.2 W/(m·K) Show Material materials with Thermal conductivity of 21.2 W/(m·K) | ||

700.0 °C | 22.8 W/(m·K) Show Material materials with Thermal conductivity of 22.8 W/(m·K) | ||

800.0 °C | 24.3 W/(m·K) Show Material materials with Thermal conductivity of 24.3 W/(m·K) | ||

900.0 °C | 25.7 W/(m·K) Show Material materials with Thermal conductivity of 25.7 W/(m·K) | ||

1000.0 °C | 27.3 W/(m·K) Show Material materials with Thermal conductivity of 27.3 W/(m·K) | ||

Unlock all property charts | |||

Thermal diffusivity | 20.0 °C | 3.1 mm²/s Show Material materials with Thermal diffusivity of 3.1 mm²/s | |

100.0 °C | 3.3 mm²/s Show Material materials with Thermal diffusivity of 3.3 mm²/s | ||

200.0 °C | 3.6 mm²/s Show Material materials with Thermal diffusivity of 3.6 mm²/s | ||

300.0 °C | 3.9 mm²/s Show Material materials with Thermal diffusivity of 3.9 mm²/s | ||

400.0 °C | 4.2 mm²/s Show Material materials with Thermal diffusivity of 4.2 mm²/s | ||

500.0 °C | 4.4 mm²/s Show Material materials with Thermal diffusivity of 4.4 mm²/s | ||

600.0 °C | 4.6 mm²/s Show Material materials with Thermal diffusivity of 4.6 mm²/s | ||

700.0 °C | 4.9 mm²/s Show Material materials with Thermal diffusivity of 4.9 mm²/s | ||

800.0 °C | 5.2 mm²/s Show Material materials with Thermal diffusivity of 5.2 mm²/s | ||

900.0 °C | 5.5 mm²/s Show Material materials with Thermal diffusivity of 5.5 mm²/s | ||

1000.0 °C | 5.7 mm²/s Show Material materials with Thermal diffusivity of 5.7 mm²/s | ||

Unlock all property charts |

Electrical

Property | Temperature | Value |
---|---|---|

Electrical resistivity | 20.0 °C | 9.9E-7 - 1.01E-6 Ω·m Show Material materials with Electrical resistivity of 9.9E-7 - 1.01E-6 Ω·m |

100.0 °C | 1.04E-6 Ω·m Show Material materials with Electrical resistivity of 1.04E-6 Ω·m | |

200.0 °C | 1.08E-6 Ω·m Show Material materials with Electrical resistivity of 1.08E-6 Ω·m | |

300.0 °C | 1.12E-6 Ω·m Show Material materials with Electrical resistivity of 1.12E-6 Ω·m | |

400.0 °C | 1.15E-6 Ω·m Show Material materials with Electrical resistivity of 1.15E-6 Ω·m | |

500.0 °C | 1.18E-6 Ω·m Show Material materials with Electrical resistivity of 1.18E-6 Ω·m | |

600.0 °C | 1.2E-6 Ω·m Show Material materials with Electrical resistivity of 1.2E-6 Ω·m | |

700.0 °C | 1.22E-6 Ω·m Show Material materials with Electrical resistivity of 1.22E-6 Ω·m | |

800.0 °C | 1.24E-6 Ω·m Show Material materials with Electrical resistivity of 1.24E-6 Ω·m | |

900.0 °C | 1.26E-6 Ω·m Show Material materials with Electrical resistivity of 1.26E-6 Ω·m | |

1000.0 °C | 1.27E-6 Ω·m Show Material materials with Electrical resistivity of 1.27E-6 Ω·m | |

Unlock all property charts |

Chemical properties

Property | Value |
---|---|

Aluminium | 0.2 - 0.5 % Show Material materials with Aluminium of 0.2 - 0.5 % |

Carbon | 0.03 - 0.08 % Show Material materials with Carbon of 0.03 - 0.08 % |

Chromium | 19 - 22 % Show Material materials with Chromium of 19 - 22 % |

Cobalt | 0.5 % Show Material materials with Cobalt of 0.5 % |

Copper | 0.5 % Show Material materials with Copper of 0.5 % |

Manganese | 1.5 % Show Material materials with Manganese of 1.5 % |

Nickel | 30 - 32.5 % Show Material materials with Nickel of 30 - 32.5 % |

Niobium | 0.1 % Show Material materials with Niobium of 0.1 % |

Phosphorus | 0.02 % Show Material materials with Phosphorus of 0.02 % |

Silicon | 0.7 % Show Material materials with Silicon of 0.7 % |

Sulfur | 0.01 % Show Material materials with Sulfur of 0.01 % |

Titanium | 0.2 - 0.5 % Show Material materials with Titanium of 0.2 - 0.5 % |